I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1
Prediction and Control of Weld Bead Geometry in Gas Metal Arc Welding Process Using Simulated Annealing Algorithm 1,
P, Sreeraj, 2,T, Kannan , 3,Subhasis Maji
1,
Department of Mechanical Engineering, Valia Koonambaikulathamma College of Engineering Technology, Kerala, 692574 India 2, Principal, SVS College of Eng ineering,Coimbatore,Tamilnadu,642109 India . 3, Professor, Depart ment of Mechanical Eng ineering IGNOU, Delhi, 110068, India.
Abstract In order to automate a welding process, which is a present trend in fab rication industry, it is necessary to have a mathematical model that is to relate the process parameters. Because of high reliability, easiness in operation, high penetration good surface finish and high productivity gas metal arc weld ing (GMAW) became a natural choice for fabrication industries. This paper presents five level factorial techniques to predict four critical d imensions of bead geometry. The developed models have been checked for adequacy and significance. The bead geometry is predicted again using Simulated annealing Algorith m (SA).
Key Words: GMAW, Weld bead geometry, Multip le Regression, Mathematical models, 1. Introduction Quality is a vital factor in today’s manufacturing world. Quality can be defined as the degree of customer satisfaction. Quality of a product depends on how it performs in desired circu mstances. Quality is a very vital factor in the field of weld ing. The quality of a weld depends on mechanical properties of the weld metal which in turn depends on metallurg ical characteristics and chemical co mposition of the weld [1]. The mechanical and metallurg ical feature of weld depends on bead geometry which is directly related to welding process parameters. In other wo rds quality of weld d epends on in process parameters.GMA welding is a mu lti objective and mult ifactor metal fabrication technique. The process parameters have a direct influence on bead geometry [2]. Fig 1 shows the clad bead geometry. Mechanical strength of clad metal is highly influenced by the co mposition of metal but also by clad bead shape. This is an indicat ion of bead geometry. It main ly depends on wire feed rate, welding speed, arc voltage etc. Therefore it is necessary to study the relationship between in process parameters and bead parameters to study clad bead geometry. Th is paper highlights the study carried out to develop mathematical and GA models to predict clad bead geometry, in stainless steel cladding deposited by GMAW [3].
Percentage dilution (D) = [B/ (A+B)] X 100 Figure 1: Clad bead geometry
2. Experimentation The following machines and consumables were used for the purpose of conducting experiment. 1) A constant current gas metal arc welding machine (Invrtee V 350 – PRO advanced processor with 5 – 425 amps output range) 2) Welding manipulator 3) Wire feeder (LF – 74 Model) 4) Filler material Stainless Steel wire of 1.2mm diameter (ER – 308 L). 5) Gas cylinder containing a mixtu re of 98% argon and 2% of o xygen. 6) Mild steel plate (grade IS – 2062) Test plates of size 300 x 200 x 20mm were cut fro m mild steel plate of grade IS – 2062 and one of the surfaces is cleaned to remove o xide and dirt before cladding. ER308 L stainless steel wire of 1.2mm d iameter was used for depositing the clad beads through the feeder. Argon gas at a constant flow rate of 16 litres per minute was used for shielding. The properties of base metal and filler wire are shown in Tab le 1. The important and most difficult parameter found fro m trial run is wire feed
Issn 22503005(online)
January 2013
Page 213
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1
rate. The wire feed rate is proportional to current. Wire feed rate must be greater than crit ical wire feed rate to achieve pulsed metal transfer. The relationship found from trial run is shown in equation (1). The formu la derived is shown in Fig 2. Wire feed rate = 0.96742857 *current + 79.1
 (1)
The selection of the welding electrode wire based on the matching the mechanical propert ies and physical characteristics of the base metal, weld size and existing electrode inven tory [4]. A candidate material for cladding which has excellent corrosion resistance and weld ability is stainless steel. These have chloride stress corrosion cracking resistance and strength significantly greater than other materials. These have good surface appearance, good radiographic standard quality and minimu m electrode wastage. Experimental design used for this study is shown in Fig 3 and importance steps are briefly explained. Table 1: Chemical Composition of B ase Metal and Filler Wire Elements, Weight % M aterials
C
SI
IS 2062
0.150
0.160
ER308L
0.03
0.57
Mn
P
S
Al
Cr
Mo
Ni
0.870
0.015
0.016
0.031



1.76
0.021
1.008

19.52
0.75
10.02
Figure 2: Relationshi p between Current and Wire Feed Rate
3. Plan of Investigation The research work is carried out in the following steps [5] .Identificat ion of factors, finding the limit of process variables, development of design matrix, conducting experiments as per design matrix, record ing responses, development of mathematical models, checking adequacy of developed models, and predicting the parameters.
3.1 Identification of Factors and Responses The basic difference between weld ing and cladding is the percentage of dilution. The properties of the cladding is the significantly in fluenced by dilution obtained. Hence control of dilution is impo rtant in cladding where a low dilution is highly desirable. When dilution is quite lo w, the final deposit composition will be closer to that of filler material and hen ce corrosion resistant properties of cladding will be great ly improved. The chosen factors have been selected on the basis to get minimal dilution and optimal clad bead geometry [1]. These are wire feed rate (W), welding speed (S), weld ing gun angle (T), contact tip to work to The following independently controllable process parameters were found to be affecting output parameters distance (N) and pinch (Ac), The responses chosen were clad bead width (W), height of reinforcement (R), Depth of Penetration. (P) and percentage of d ilution (D). Th e responses were chosen based on the impact of parameters on final composite model. 3.2 Findi ng the limi ts of process vari ables Working ranges of all selected factors are fixed by conducting trial run. This was carried out by varying one of factors while keeping the rest of them as constant values. Working range of each process parameters was decided upon by inspecting the bead for smooth appearance without any visible defects. The upper limit of given factor was coded as 2. The coded value of intermediate values were calculated using the equation (2)
Issn 22503005(online)
January 2013
Page 214
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1
=
 (2)
Where Xi is the required coded value of parameter X is any value of parameter fro m of parameters and Xmax is the upper limit parameters [4]. The chosen level of the parameters with their un its and notation are given in Table 2.
X min â€“ X max. Xmin is the lower limit
Table 2: Wel ding Parameters and their Levels Parameters
Factor Levels Unit
Notation
2
1
0
1
2
Welding Current
A
1
200
225
250
275
300
Welding Speed
mm/min
S
150
158
166
174
182
Contact tip to work distance
mm
N
10
14
18
22
26
Welding gun Angle
Degree
T
70
80
90
100
110
Pinch

Ac
10
5
0
5
10
3.3 Devel opment of design matrix Design matrix chosen to conduct the experiments was central co mposite rotatable design. The design matrix comprises of full replication of 25 (= 32), Factorial designs. All weld ing parameters in the intermediate levels (o) Constitute the central points and combination o f each welding parameters at either is highest value (+2) or lowest (2) with other parameters of intermediate levels (0) constitute star points. 32 experimental t rails were conducted that make the estimation of linear quadratic and two way interactive effects of process parameters on clad geometry [5].
Figure 3: GMAW Circuit Di agram Table 3: Design Matrix Trial Number 1 2
I 1 1
S 1 1
3
1
1
4
1
5
Design M atrix N 1 1
T 1 1
Ac 1 1
1
1
1
1
1
1
1
1
1
1
1
1
6
1
1
1
1
1
7
1
1
1
1
1
8
1
1
1
1
1
9
1
1
1
1
1
10
1
1
1
1
1
Issn 22503005(online)
January 2013
Page 215
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1 11
1
1
1
1
1
12
1
1
1
1
1
13 14 15 16
1 1 1 1
1 1 1 1
1 1 1 1
1 1 1 1
1 1 1 1
17
2
0
0
0
0
18
2
0
0
0
0
19
0
2
0
0
0
20
0
2
0
0
0
21 22
0 0
0 0
2 2
0 0
0 0
23 24
0 0
0 0
0 0
2 2
0 0
25 26
0 0
0 0
0 0
0 0
2 2
27 28
0 0
0 0
0 0
0 0
0 0
29 30
0 0
0 0
0 0
0 0
0 0
31 32
0 0
0 0
0 0
0 0
0 0
I  Wel ding current; S  Wel ding s peed; N  Contact ti p to work distance; T  Wel ding gun angle; Ac â€“ Pinch 3.4 Conducting experi ments as per design matri x In this work Thirty two experimental run were allo wed for the estimation of linear quadratic and two way interactive effects of correspond each treat ment co mb ination of parameters on bead geo metry as shown Table 3 at rando m. At each run settings for all parameters were d isturbed and reset for next deposit. This is very essential to introduce variability caused by errors in experimental set up. The experiments were conducted at SVS College of Engineering, Coimbatore, 642109, India. 3.5 Recordi ng of Responses For measuring the clad bead geo metry, the transverse section of each weld overlays was cut using band saw fro m mid length. Position of the weld and end faces were machined and grinded. The specimen and faces were polished and etched using a 5% nital solution to display bead dimensions. The clad bead profiles were t raced using a reflective type optical prof ile projector at a magnification of X10, in M/s Roots Industries Ltd. Coimbatore. Then the bead dimension such as depth of penetration height of reinforcement and clad bead width were measured [6]. The profiles traced using AUTO CAD software. This is shown in Fig 4. Th is represents profile of the specimen (front side).The cladded specimen is shown in Fig. 5. The measured clad bead dimensions and percentage of dilution is shown in Table 4.
Figure 4: Traced Profile of bead geometry
Issn 22503005(online)
January 2013
Page 216
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1
Figure 5: cl added s pecimen Table 4: Design Matrix and Observed Values of Clad Bead Geometry W
Trial No.
Design Matrix
Bead Parameters
1 2 3 4 5 6 7 8 9 10 11 12 13 14 15 16 17 18 19 20 21 22
I 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 2 2 0 0 0 0
S 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 0 0 2 2 0 0
N 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 0 0 0 0 2 2
T 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 0 0 0 0 0 0
Ac 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 1 0 0 0 0 0 0
W (mm) 6.9743 7.6549 6.3456 7.7635 7.2683 9.4383 6.0823 8.4666 6.3029 7.0136 6.2956 7.741 7.3231 9.6171 6.6335 10.514 6.5557 7.4772 7.5886 7.5014 6.1421 8.5647
P (mm) 1.67345 1.9715 1.6986 1.739615 2.443 2.4905 2.4672 2.07365 1.5809 1.5662 1.58605 1.8466 2.16475 2.69495 2.3089 2.7298 1.99045 2.5737 2.50455 2.1842 1.3752 3.18536
R (mm) 6.0262 5.88735 5.4519 6.0684 5.72055 5.9169 5.49205 5.9467 5.9059 5.9833 5.5105 5.8752 5.72095 6.37445 5.554 5.4645 5.80585 6.65505 6.4069 5.6782 6.0976 5.63655
D (% ) 10.72091 12.16746 12.74552 10.61078 16.67303 15.96692 16.5894 14.98494 10.2749 9.707297 11.11693 11.4273 15.29097 18.54077 17.23138 20.8755 13.65762 15.74121 15.77816 16.82349 8.941799 22.94721
23 24 25 26 27 28 29 30 31 32
0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0
0 0 0 0 0 0 0 0 0 0
2 2 0 0 0 0 0 0 0 0
0 0 2 2 0 0 0 0 0 0
7.9575 7.7085 7.8365 8.2082 7.9371 8.4371 9.323 9.2205 10.059 8.9953
2.2018 1.85885 2.3577 2.3658 2.1362 2.17145 3.1425 3.2872 2.86605 2.72068
5.8281 6.07515 5.74915 5.99005 6.0153 5.69895 5.57595 5.61485 5.62095 5.7052
15.74941 13.27285 16.63287 16.38043 15.18374 14.82758 22.8432 23.6334 21.55264 19.60811
Width; R  Reinfo rcement W  Width; P  Penetration; D  Dilution % 3.6 Devel opment of Mathematical Models The response function representing any of the clad bead geometry can be expressed as [7, 8, and 9], Y = f (A, B, C, D, E) Where, Y = Response variable A = Welding current (I) in amps B = Welding speed (S) in mm/ min
Issn 22503005(online)
 (3)
January 2013
Page 217
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1
C = Contact tip to Work distance (N) in mm D = Welding gun angle (T) in degrees E = Pinch (Ac) The second order surface response model equals can be expressed as below
Y = β 0 + β 1 A + β 2 B + β 3 C + β 4 D + β 5 E + β 11 A2 + β22 B2 + β 33 C2 + β 44 D2 + β 55 E2 + β12 AB + β 13 AC + β 14 AD + β 15 AE + β 23 BC + β 24 BD + β 25 BE + β 34 CD + β35 CE+ β 45 DE  (4) Where, β 0 is the free term of the regression equation, the coefficient β 1 , β2 , β3 , β4 and β5 is are linear terms, the coefficients β 11 , β 22 , β33 , β44 and ß 55 quadratic terms, and the coefficients β 12 , β13 , β14 , β15 , etc are the interaction terms. The coefficients were calculated by using Quality A merica six sig ma software (DOE – PC IV). After determining the coefficients, the mathemat ical models were developed. The developed mathematical models are g iven as follo ws.  (5)  (6)  (7)  (8) Clad Bead Wi dth (W), mm = 8.923 + 0.701A + 0.388B + 0.587C + 0.040D + 0.088E – 0.423A 2 – 0.291B2 – 0.338C2 – 0.219D2 – 0.171E2 + 0.205A B + 0.405AC + 0.105AD + 0.070A E– 0.134BC+0.225BD+0.098BE+0.26CD+0.086CE+0.012DE  (9) Depth of Penetration (P), mm = 2.735 + 0.098A – 0.032B + 0.389C – 0.032D – 0.008E – 0.124A 2 – 0.109B2 – 0.125C2 – 0.187D2 – 0.104E2 – 0.33AB + 0.001 AC + 0.075AD + 0.005 AE– 0.018BC+0.066BD+0.087BE+0.058CD+0.054CE– 0.036DE  (10) Height of Reinforcement (R), mm = 5.752 + 0.160A – 0.151B – 0.060C + 0.016D – 0.002E + 0.084A 2 + 0.037B2 – 0.0006C2 + 0.015D2 – 0.006E2 + 0.035A B + 0.018AC – 0.008AD – 0.048A E– 0.024BC–0.062BD–0.003BE+0.012CD– 0.092CE–0.095DE.(11) Percentage Dilution (D), % = 19.705 + 0.325A + 0.347B + 3.141C – 0.039D – 0.153E – 1.324A 2 – 0.923B2 – 1.012C2 – 1.371D2 – 0.872E2 – 0.200AB + 0.346 AC + 0.602 AD + 0.203A E+0.011BC+0.465BD+0.548BE+0.715CD+0.360CE+0.137DE  (12) Coefficient of the above polynomial equation where calculated by reg ression as given by equations (5) to (8) 3.7 Checking the adequacy of the developed models Analysis of variance (ANOVA) technique was used to test the adequacy of the model. As per this technique, if the F – ratio values of the developed models do not exceed the standard tabulated values for a desired level of confidence (95%) and the calculated R – ratio values of the developed model exceed the standard values for a desired level of confidence (95%) then the models are said to be adequate within the confidence limit [10]. These conditions were satisfied for the developed models. The values are shown in Table 5.
Paramete r
Table 5: Anal ysis of variance for Testing Adequacy of the Model 2 nd order 1 st Order terms Lack of fit Error terms Fterms ratio SS DF SS DF SS DF SS DF
Rratio
Whether model is adequate
W
36.889
20
6.233
11
3.51 3
6
2.721
5
1.076
3.390
Adequate
P
7.810
20
0.404
11
0.142
6
0.261
5
0.454
7.472
Adequate
R
1.921
20
0.572
11
0.444
6
0.128
5
2.885
3.747
Adequate
D
506.07 4
20
21.73 9
11
6.289
6
15.45
5
0.339
8.189
Adequate
SS  Sum of squares; DF  Degree of freedom; F Ratio (6, 5, 0.5 ) = 3.40451; R Ratio (20, 5, 0.05) = 3.20665
4. The Prediction Function The mathematical models furn ished above provide one to one relationships between process parameters and weld bead geometry. They can be used in two ways;
Issn 22503005(online)
January 2013
Page 218
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1
1) Pred icting weld bead geometry based on in p u t p a ramet ers an d 2) Pred ict in g p ro cess parameters for a desired weld bead specification. The later o ne is mo re p ract ical s in ce t he weld ing parameters are usually set based on desired bead geometry. For this purpose, the set of nonlinear equations must be solved simultaneously for all the process parameters. Evolutionary algorith ms are powerful optimization techniques widely used for solving combinatorial problems. Nevertheless, other capabilit ies of these techniques have rarely been explored. As a new and promising approach, one of these algorith ms, called SA , is implemented for prediction purposes in this research. To predict the process parameters based on a desired bead quality, we first define the prediction function as follow(13): E=
+
………………………………………………………..
(13) Where: are bead specifications namely penetration, reinforcement, width of weld bead and percentage of dilution respectively which are given by Equations 9 to 12. In the same manner, we define as the targ et valu es for the desired weld bead geometry. The coefficients represent weighing importance of different parameters in the objective function. In the prediction process, the purpose is to min imize this o b ject iv e fun ct io n . By d o in g so , th e p rocess parameters are calculated in such way that the bead geometry parameters approach their desired values. A SA method is emp loyed to find the best weld ing variables with respect to process specifications.
5. Simulated Annealing Algorithm Simu lated annealing was originally inspired by formation of a crystal in s olids during cooling. As discovered by long ago by Iron Age black s miths the slower cooling, the most perfect crystal is formed. By cooling co mplex physical systems naturally converge towards state of minimal energy. The systems move randomly, but probability to stay in a particular configuration depends directly on the energy of the system and on its temperature. Gibbs law stated as equation (14). P=  (14) Where E stands for energy k is the Bolt zmann constant and T is the temperature. The iterat ion of the simulated annealing consists of randomly choosing a new solution in the neighbourhood of actual solution. If the fitness function of the new solution is better than the fitness function of the current one the new solution is accepted as the new current solution. If the fitness function is not improved the new solution will be retained with p robability shown in equation (15). P=  (15) Where f(y)f(x), being the difference between new and old solutions. In this study Simulated Annealing (SA) which utilizes stochastic optimizat ion is used for the optimizat ion of clad bead geometry deposited by GMAW. The main advantage of using this stochastic algorithm is that global optimizat ion point can be reached regardless of the initial starting point. Since the algorith m incorporates. The major advantage of SA is an abilit y to avoid being trapped at a local optimu m point during optimization. The algorith m emp loys a random search accepting not only the changes that improve the objective function but also the changes that deteriorate it.Fig.6 shows simu lated annealing algorith m. [11]
Issn 22503005(online)
January 2013
Page 219
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1
Figure. 6 Trad itional Simulated Annealing A lgorith ms
6 An Illustrative Example In this section a numerical example is presented to illustrate the performance of proposed procedure and solution technique [12]. The target values for desired weld bead geometry are given in Table 6. Table 6 Target values for weld bead geometry. Weld Bead Geometry
Target Value
Pt , (mm)
2.49
Rt (mm)
5.83
Wt (mm)
7.99
D t (%)
12.59
Without lose of generality, all elements of the bead geometry are assumed to be of the same importance and therefore constants al to a7 are set to unity [13]. The prediction function given in Equation 13 along wit h weld bead mo deling eq uat ions 9 to 12 are embedded into SA algorithm. The parameters for the algorithm are set as follows and shown in Table 7: Table 7. SA process parameters Annealing Function Population size Re annealing temperature Initial Temperature Data Type
Bolt zmann Annealing 30 100 100 Double
The objective is to minimize the perdition function which is used as the fitness criterion in evaluation each generation of solutions. The best values found by proposed SA for process parameters are presented in Table 8. By setting these parameters in GMAW, the target weld bead geometry specificat ions may be achieved.
Issn 22503005(online)
January 2013
Page 220
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1
Table 8 Predicted values for process parameters. Process parameters
Predicted value by S A
Welding current (I)
242
Welding Speed (S) (mm/min)
161
Contact tip to work distance (N) mm (m/min)
16
Welding Gun Angle (T) Degree
88
Pinch(Ac)
10
The performance of the solution procedure was tested by substituting parameters values obtained by GA into the weld bead models and comparing the results with the des ired valu es of bead geo met ry. The co mparison of the calculated and desired values is shown in Table 9. The largest error is around 0.3 while most parameters deviate much less than 1% from their desired values. The computational results show that GA can be used efficiently and with good accuracy as a prediction technique. Table 9 Comparison between desired and predicted weld bead geometry values Weld Bead Geometry
Targets
S AResults
Error
Penetration
2.29
2.493
.203
Reinforcement
5.83
6.213
.383
Clad Bead Width
7.9
8.35
.45
Clad Bead Width
7.9
8.35
.45
7. Results and Discussions 1. A five level five factor fu ll factorial design matrix based on central co mposite rotatable design technique was used for the mathematical development of model to predict clad bead geometry of austenitic stainless steel deposited by GMAW. 2. SA tool available in MATLA B 7 software was efficiently emp loyed for pred iction of clad bead geometry. 3. In cladding by a weld ing process clad bead geometry is very important for economising the material. Th is study effectively used SA models to predict weld bead geometry. 4. In this study two models regression and SA system for prediction of bead geometry in GMAW welding process. In this study it is proved that SA model pred iction is efficient and error is appro ximately equal to five percent.
8. Conclusions Based on the above study it can be observed that the developed model can be used to predict clad bead geo metry within the applied limits of process parameters. This method of predicting process parameters can be used to get minimu m percentage of dilution. In this study regression and SA was used for achieving optimal clad bead dimensions. In the case of any cladding process bead geometry plays an important role in determining the properties of the surface exposed to hostile environments and reducing cost of manufacturing. In this approach the objective function aimed for predicting weld bead geometry within the constrained limits.
Acknowledgement The authors sincerely acknowledge the help and facilities extended to them by the department of mechanical engineering SVS college of Eng ineering, Co imbatore, India .
References [1] [2] [3] [4] [5]
Kannan,T.;M urugan,N.(2006).Effect Of Flux Cored Arc Welding Process Parameters On Duplex Stainless Steel Clad Quality ,Journal Of M aterial Processing Technology Vol.176 Pp 230239. Kannan,T.; M urugn,N.(2006).Prediction Of Ferrite Number Of Duplex Stainless Steel Clad M etals Using RSM , Welding Journal. Pp. 91  99. Gunaraj,V.; M urugan, N. (2005). Prediction And Control Of Weld Bead Geometry And Shape Relationships In Submerged Arc Welding Of Pipes, Journal Of Material Processing Technology. Vol. 168, Pp. 478 â€“ 487. Kim, I,S.; Son, K,J.; Yang, Y, S.; Yaragada, P, K, D,V. (2003). Sensitivity Analysis For Process Parameters In GM A Welding Process Using Factorial Design M ethod, International Journal Of Machine Tools And Manufacture. Vol.43, Pp. 763  769. Cochran, W,G.; Coxz, G,M . (1987). Experimental Design. Pp.370, New York, John Wiley & Sons.
Issn 22503005(online)
January 2013
Page 221
I nternational Journal Of Computational Engineering Research (ijceronline.com) Vol. 3 Issue. 1 [6] [7] [8] [9] [10] [11] [12] [13]
Serdar Karaoglu.; Abdullah Secgin. (2008). Sensitivity Analysis Of Submerged Arc Welding Process Parameters,Journal Of Material Processing Technology. Vol202, Pp 500507. Ghosh, P,K.; Gupta, P,C.; Goyal, V,K. (1998) . Stainless Steel Cladding Of Structural Steel Plate Using The Pulsed Current GM AW Process, Welding 314. Gunaraj, V.; M urugan, N. (1999) . Prediction And Comparison Of The Area Of The Heat Effected Zone For The Bead On Plate And Bead On Joint In SAW Of Pipes, Journal Of Material Processing Technology. Vol. 95, Pp. 246  261. M ontgomery, D,C.; (2003). Design And Analysis Of Experiments, John Wiley & Sons (ASIA) Pvt. Ltd. Kannan,T.; Yoganath. (2010). Effect Of Process Parameters On Clad Bead Geometry And Shape Relationships Of Stainless Steel Cladding Deposited By GM AW, Int. Journal Of Manufacturing Technology. Vol47, Pp 10831095. Deepa,S,N;Sivanandam,S,N.;Introduction To Genetic Algorithms;Springer ;Spin 12053230. Farhad Kolahan.; M ehdi Heidari; (2010). A New Approach For Predicting And Optimising Weld Bead Geometry In GMAW, International Journal Of Mechanical System Science And Engineering, 2:2: Pp.138 142. M ostafa, N,B.;Khajavi, M ,N.(2006).Optimization Of Welding Parameters For Weld Penetration In FCAW, Journal Of Achievements In Materials And Manufacturing Engineering, Vol16 Issue 12 M ay June.
Issn 22503005(online)
January 2013
Page 222